View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
TABLE OF CONTENT Mobile Flash Butt Welding Uses of Mobile Flash Butt Welding Various Options in Mobile Flash Butt Welding Staff Requirement for Mobile Flash Butt welding Mobile Flash Butt Welding Procedure Pre Welding Checks Actual Welding Procedure Testing of Welds Precautions in Mobile Flash Butt Welding
Mobile Flash Butt Welding Mobile Flash Butt Welding is a Rail cum Road Machine. Mobile Flash Butt Welding Plant is a four wheeled mobile vehicle, which can travel on roads with rubberised wheels and on rails with metal wheels in which the following are fitted: Welding Equipment Welding Parameter Recorder Separate units for Grinding & USFD Testing Equipment
Mobile Flash Butt Welding Plant moving on track
Unloading the welding Equipment from the vehicleModel AMS60 Made Schlatter
Unloading the welding Equipment from the vehicleModel K-920 Holland Made
Uses of Mobile Flash Butt Welding The basic use of the Mobile Flash Butt Welding is to use the flash butt welding technique in field which otherwise cannot be done using the static plant. The Mobile Flash Butt Welding is preferable as the welds have much better fatigue strength and performance as compared to the AT welding otherwise used. It is basically used for the following purposes: In construction works for converting free rails or 3 rail panels (which is the maximum possible to be laid in new lines due to transportation constraints) to LWR. In open Line for Through Weld renewal to replace welds which have completed their life.
Various Options in Mobile Flash Butt Welding FIXED SITE DEPOTS MOBILE DEPOTS MOBILE FBW PLANT
The different options have their own advantages & disadvantages: SL No FIXED SITE DEPOTS MOBILE DEPOTS MOBILE FBW PLANT 1 Panels can be made at At convenient locations, the Plant moves and reaches one point only. depots can be setup and the every point of welding. Transportation has to panels will require to be be done. transported from this location only. 2 Time for welding is Time for welding is min but Time for welding less. Time for setting up of plants takes maximum as plant to be transportation of some time at each location. setup for each weld. No panels maximum. Transportation of panels transportation of panels. takes lesser time. 3 Suitable for smaller Suitable for construction Suitable for construction lengths of track where projects if the welding work projects if the track one set up can serve to form panels is to be done in possession can be given for the entire stretch in parallel with the other works. the plant to work. Work construction as well as In open line, suitable for TWR will commence only after open line. and the plant can be setup the rails are laid on near any level crossing or completed formation. approachable location.
Staff Requirement for Mobile Flash Butt welding The Welding team may consist of one Supervisor and two welders. The educational qualification of the Supervisor should be minimum Diploma in Mechanical / Electrical Engg. or B.Sc and that of welder should be minimum Class X or equivalent pass. Zonal Railways should ensure periodic training of welders on Mobile Flash Butt Welding Plant. The competency certificate of welder of Mobile Flash Butt Welding Plant is issued by the Zonal Railways.
The Supervisor and Welder of the Plant should haveacquaintance in knowledge of the following. Welding parameters and its influence on quality of welding and heat affected zone Suitability of rails for welding Preparation of rails to be welded including pre straightening of rails Procedure of welding of rails Record of welds Post weld straightening of rails Finishing of joints Marking of joints Testing of welds Precautions to avoid defects in rail joints
Mobile Flash Butt Welding Procedure There are three basic mechanisms in the machine: CLAMPING MECHANISM FORGING MECHANISM TRANSFORMER
The Schematic representation of a Mobile Flash ButtWelding unit is as follows:
Basic Principle of Flash Butt Welding The basic principle is that heat is generated by electric resistance method at the ends of two rails to be welded which were firmly clamped into the jaws of the welding machine. Both the jaws of the machine are movable and as such, the gap between the two rail ends can be adjusted.
Pre Welding Checks Preparation of rails before welding: In construction work, the free rails transported to the site of work are placed over the uniformly spaced sleepers over the ballast bed on the formation, without clipping them with the sleepers, with their ends are butt each other. In open line, 7 sleepers on either side of the weld are to be opened out for the welding process.
Straightening & Cleaning of rail ends Straightening of rails : The rails ends are required to be straightened with the help of hydraulic rams before welding so as to get good alignment of the welded rail . Cleaning of rail ends: The rail ends shall be cleaned using grinders to get clean surface.
Inspection of Rail ends A thorough inspection of rail ends shall be carried out and the deviation of vertical and horizontal misalignment should be within the tolerable limits as given below: Individual welded ends may have a maximum difference in height of 1.2 mm as in case of second hand rails.
If the rail wear is not equal, the grouping of rails so that maximum difference of height doesnot exceed 1.2 mm shall be done as shown in figure
Welding of second hand rails Second hand rails within the following limit of tolerance can also be welded using Mobile Flash Butt Welding: Rail New Rail Second Hand Rail 60Kg 172.00 mm 164 mm 52Kg 156.00 mm 150 mm 90R 142.88mm 139 mm Rail New Rail Second Hand Rail 60Kg 72.00 mm 66 mm 52Kg 67.00 mm 61 mm 90R 66.68mm 61 mm The tolerance on the end bends in the vertical plane should be (+) 0.7mm and (-) 0.0mm on a straight edge of 1.5 m.
Tolerances for rail in vertical plane The tolerance on the end bends in the horizontal plane should be (+) or (-) 0.7mm on a straight edge of 1.5 m.
Tolerances specified for rail ends The dimensions of the head width of rail should be checked and should be less than 0.5 mm deviation
Tolerances for rail ends The rail ends shall be cut vertically and these shall be as per tolerances given below:
Actual Welding Procedure Clamping the rail ends: The mobile flash butt welding machine is lowered from the vehicle and the rail ends which are close together are clamped. The The rail ends are then brought together so that almost touch each other to create the flash. The longitudinal and vertical alignment of the rail is corrected by suitable adjustments of the machine. The rail ends being clamped by the welding machine
The rail ends being clamped by the welding machine
The rail ends clamped and welding process about tobegin
Close up view of the rail ends clamped by thewelding machine
Setting up the flash The rails are brought towards each other till the flash starts. The flash will lead to heat generation which will soften the steel. The electric energy is switched on and thereby allowing and electric current of about 5 volts and 35,000 Amperes to pass between interfaces of two rails. Lot of flashing takes place and considerable heat is generated by the passage of electric current between the rail ends. The rail ends are moved to and fro automatically by the machine till the temperature rises to the fusion limits in the range of 1000° C to 1500° C.
Applying force The rail ends are then hydraulically pressed so that the softened rail ends fuse together to form weld. At this juncture, the rail ends are pressed together with an upset pressure of about 37 T. The final flashing takes place joining the two rail ends together. The welding is so regulated that any steel that might have been oxidized during the heating process gets completely squeezed out.
Stripping the weld As soon the rails are welded, they are made to pass through a stripping Unit where all the extra metal called upsets is chipped off. The removal of metal by stripping is so good that except the head no other portion require any finishing.
Weld completedThe average time taken for welding a joint is about 6 minutes per joint and No.of joints that can be welded is about 50 to 55 joints per 8 hrs shift.
Grinding rail endsThe rail table and gauge face of the joints thus welded, arefinally ground to correct rail profile, by means of a trolleygrinder for the rail table and by pneumatic grinders for otherportions.
Post straightening & Ultrasonic TestingPost straightening: The rails are post straightened mechanically to removehorizontal and vertical kinks so as to give perfect alignment in both directions.Ultrasonic Testing: The welded rails are then ultrasonically tested with normal 70°and 45° probes.
Weld numbering and identificationEach weld shall be given a number so as to identify the weld, welder andcorrelation can be established between the field weld and the weld record. Testing of Welds Weld recorder: The machine has a weld recorder which measures and stores the welding parameters. The results are stored in machine and can be retrieved later on also. Print out can also be obtained of the welding parameters which can be used as permanent record. The following parameters are recorded (figures in brackets are standard values): Pre Flash Time (47 sec) Flash Time (95 sec) Boost Time (07 sec) Up set Time (1.8 sec) Forge Time (2 sec) Current Set (190 – 280 Amps) Forge Force (38 – 65 Tons) Up set Rail Use (12.7 mm) Welding parameters will depend on section and metallurgy of rail to be welded. These are, normally, specified by the manufacturer of the plant. Before adoption, the welding parameters shall be got approved from RDSO. RDSO shall consider parameters suggested by the manufacturer while fixing the parameters.
Standardized for Flash Butt Welding Plant Zonal Railways / Owner of Mobile Flash Butt Welding Plant are required to get the welding parameters standardized for their Flash Butt Welding Plant for different rail chemistry and rail section in consultation with RDSO, Lucknow before regular operation of the plant. RDSO will standardize welding parameters for a particular machine, make and model. These standardized parameters shall be circulated to Zonal Railways and shall be applicable for same type of machine working on other Zonal Railways also. For Mobile Flash Butt Welding Plant of particular make for which standardized parameters exist, sample testing will be carried out either at RDSO or at the nearest Flash Butt Welding Plant (having the testing facilities) in presence of RDFSO official to check the compliance of machine. For all Mobile Flash Butt Welding Plants, QAP will be approved by RDSO before plant is put to regular operation. The welding parameters should be available with welder of the plant and displayed at appropriate point on the plant. Following tests shall be conducted on the welds:
Testing of Flash Butt Welded Joints Hardness Test: Brinnel hardness test shall be conducted on the test weld sample before conducting transverse load test. The hardness value in HAZ shall not vary from the hardness of the parent rail by more than + 20 HB. Results shall be maintained as per proforma given in Annexure – VI C. Extent of heat affected zone (max value in mm) Head 38 mm Web 39 mm Foot 36 mm The results of tests shall be maintained. VALUES OF MINIMUM BREAKING LOAD AND DEFLECTION IN TRANSVERSE LOAD TEST:
Testing Frequency of Flash Butt Welded Joints “Sample joints for first 1000 Joints welded by a Mobile Flash butt welding plant will be tested at a frequency of 1in 100 joints and subsequently at a frequency of 1 in 500 joints.” As Per RDSO Manual Rail section Span Min. Min. Frequency of testing Breaking Deflection Load (tones) At StationaryRDSO Manual As per Mobile & plant FBWP centre(mm)60 Kg. (UIC) NHH 1.25m 115 30 1 IN 500 1 in 10060 Kg (UIC) Cr. Mn. 1.25m 110 12 1 IN 500 1 in 100Alloy steel60 Kg. UIC (90 UTS) 1m 150 20 1 in 1000 1 in 10052 kg. 90 UTS 1m 100 15 1 in 1000 1 in 10060 Kg (UIC) MM (72 1m 135 30 1 in 1000 1 in 100UTS)52 Kg MM (72 UTS) 1m 100 30 1 in 1000 1 in 10090R MM (72 UTS) 1m 80 30 1 in 1000 1 in 10075R MM (72 UTS) 1m 70 30 1 in 1000 1 in 10060R MM (72 UTS) 1m 60 25 1 in 1000 1 in 100
Testing of Flash Butt Welded Joints Macro Examination test: One test joint for every 1000 joints welded in case of mobile flash butt welding plant shall be subjected to macro examination. 150 mm length of rail with weld at centre shall be cut and the sample shall be sectioned in vertical, longitudinal directions through the weld. One of the sections shall be etched with 5 – 10% Nitric acid and also subjected to magna flux test to ensure freedom fro cracks, lack of fusion or oxide inclusion. Extent of heat affected zone shall be measured for head, foot and web of the rail. These values should not be more than the values achieved during standardization of welding parameters of the particular rail section and chemistry of particular make of FBW Plant. Results shall be maintained as per proforma.
Precautions in Mobile Flash Butt Welding End squareness of rail faces must be ensured. Better weld strength with minimum value and merely parallel shape of heat affecting zone can be achieved using perfect matching of rail ends. Secondary out put of current should be sufficient enough to achieve complete fusion of butting faces. Butting stroke should be sufficient for complete coalescence (not less than 12 mm) Throughout Uniform and smooth auto trimming of the squeezed out metal and complete grinding using profile grinder. Minimum and nearly parallel heat affected zone of the joint should be achieved. Facilities for auto recording of weld parameters including final butting pressure shall be available. When weld is carried out in situ, minimum 20 minutes time after trimming is required to pass the first train through the weld with proper packing and support below the joint. Track should be levelled. Excess butting pressure leads to high joints. These are strictly prohibited and shall be closely monitored by trained departmental staff. To avoid buckling of track, the continuous welding is prohibited in skeleton track and a gap should be left at every 500 m interval which will be used for destressing. (In new line works) Night welding and welding during rainy session to be avoided as far as possible for obtaining better results. Target should not be fixed more than 40 joints per working day in order to keep sufficient time gap before moving allowing the machine over the newly welded joints.(In new line works) Computer printout has to be obtained for each weld just after the execution in order to rectify the variations in various parameters as recommended before commencement of the next joint..